LMucko/crystallography-open-database huggingface dataset:
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A4 - DJ102 N.12
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004415
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A4 - DJ102 N.12
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al1.58 Ca0.8 F1.02 Fe1.69 H0.98 Mg2.43 Na5.2 O22.98 Si7.28 Ti0.02'
_chemical_name_mineral           Fluor-taramite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.33
_cell_angle_gamma                90
_cell_length_a                   9.722
_cell_length_b                   17.862
_cell_length_c                   5.319
_cell_formula_units_Z            2
_cell_volume                     894.929
_cod_original_formula_sum
'Si7.28 Al1.58 Mg2.43 Fe1.69 Ti.02 Ca.8 Na5.2 H.98 O22.98 F1.02'
_cod_database_code               9004415
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A5 - G230F N.3
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004416
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A5 - G230F N.3
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al2 Ca1.06 Fe0.9 H2 Mg2.94 Na4.94 O24 Si7.12 Ti0.04'
_chemical_name_mineral           Taramite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.83
_cell_angle_gamma                90
_cell_length_a                   9.772
_cell_length_b                   17.853
_cell_length_c                   5.310
_cell_formula_units_Z            2
_cell_volume                     895.522
_cod_original_formula_sum
'Si7.12 Al2 Mg2.94 Fe.9 Ti.04 Ca1.06 Na4.94 H2 O24'
_cod_database_code               9004416
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A6 - Q99 N.3
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004417
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A6 - Q99 N.3
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al2.16 Ca1.2 Fe1.48 H2 Mg2.34 Na4.74 O24 Si7.04 Ti0.04'
_chemical_name_mineral           Taramite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.9
_cell_angle_gamma                90
_cell_length_a                   9.790
_cell_length_b                   17.899
_cell_length_c                   5.319
_cell_formula_units_Z            2
_cell_volume                     900.715
_cod_original_formula_sum
'Si7.04 Al2.16 Mg2.34 Fe1.48 Ti.04 Ca1.2 Na4.74 H2 O24'
_cod_database_code               9004417
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A7 - D163 N.2
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004418
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A7 - D163 N.2
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al1.98 Ca1.12 F0.26 Fe1.4 H1.74 Mg2.42 Na4.8 O23.74 Si7.24 Ti0.04'
_chemical_name_mineral           Katophorite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.64
_cell_angle_gamma                90
_cell_length_a                   9.737
_cell_length_b                   17.875
_cell_length_c                   5.314
_cell_formula_units_Z            2
_cell_volume                     894.867
_cod_original_formula_sum
'Si7.24 Al1.98 Mg2.42 Fe1.4 Ti.04 Ca1.12 Na4.8 H1.74 O23.74 F.26'
_cod_database_code               9004418
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A8 - D167 N.1
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004419
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A8 - D167 N.1
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al1.84 Ca1.26 F0.36 Fe1.82 H1.64 Mg2.34 Na4.56 O23.64 Si7.16 Ti0.02'
_chemical_name_mineral           Katophorite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.69
_cell_angle_gamma                90
_cell_length_a                   9.775
_cell_length_b                   17.928
_cell_length_c                   5.313
_cell_formula_units_Z            2
_cell_volume                     900.648
_cod_original_formula_sum
'Si7.16 Al1.84 Mg2.34 Fe1.82 Ti.02 Ca1.26 Na4.56 H1.64 O23.64 F.36'
_cod_database_code               9004419
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A9 - BM47 N.1
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004420
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A9 - BM47 N.1
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al1.12 Ca1.48 Cr0.28 F0.06 Fe0.73 H1.94 Mg3.69 Na4.36 O23.94 Si7.24 Ti0.1'
_chemical_name_mineral           Pargasite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.08
_cell_angle_gamma                90
_cell_length_a                   9.870
_cell_length_b                   17.991
_cell_length_c                   5.291
_cell_formula_units_Z            2
_cell_volume                     907.175
_cod_original_formula_sum
'Si7.24 Al1.12 Mg3.69 Fe.73 Ti.1 Cr.28 Ca1.48 Na4.36 H1.94 O23.94 F.06'
_cod_database_code               9004420
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A10 - FE129 N.1
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004421
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A10 - FE129 N.1
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al1.85 Ca0.98 Fe0.76 H2 Mg3.41 Na4.9 O24 Si7.08 Ti0.02'
_chemical_name_mineral           Pargasite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.17
_cell_angle_gamma                90
_cell_length_a                   9.839
_cell_length_b                   17.963
_cell_length_c                   5.291
_cell_formula_units_Z            2
_cell_volume                     902.535
_cod_original_formula_sum
'Si7.08 Al1.85 Mg3.41 Fe.76 Ti.02 Ca.98 Na4.9 H2 O24'
_cod_database_code               9004421
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A11 - FE229 N.18
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004422
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A11 - FE229 N.18
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al1.9 Ca1.78 Cr0.04 F0.04 Fe0.49 H1.96 Mg3.69 Na4.04 O23.96 Si7.04 Ti0.02'
_chemical_name_mineral           Pargasite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.33
_cell_angle_gamma                90
_cell_length_a                   9.854
_cell_length_b                   17.931
_cell_length_c                   5.282
_cell_formula_units_Z            2
_cell_volume                     900.080
_cod_original_formula_sum
'Si7.04 Al1.9 Mg3.69 Fe.49 Ti.02 Cr.04 Ca1.78 Na4.04 H1.96 O23.96 F.04'
_cod_database_code               9004422
Sodium at the A site in clinoamphiboles: the effects of composition on patterns of order Sample: A12 - KP N.1
Hawthorne F C; Oberti R; Sardone N; The Canadian Mineralogist 34 (1996) 577–593; doi:

data_9004423
_publ_section_title
;
 Sodium at the A site in clinoamphiboles: the effects of composition
 on patterns of order
 Sample: A12 - KP N.1
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              577
_journal_page_last               593
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum
'Al2.04 Ca1.76 F0.04 Fe0.69 H1.96 Mg3.23 Na4.24 O23.96 Si7.04'
_chemical_name_mineral           Pargasite
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.28
_cell_angle_gamma                90
_cell_length_a                   9.862
_cell_length_b                   17.928
_cell_length_c                   5.295
_cell_formula_units_Z            2
_cell_volume                     903.093
_cod_original_formula_sum
'Si7.04 Al2.04 Mg3.23 Fe.69 Ca1.76 Na4.24 H1.96 O23.96 F.04'
_cod_database_code               9004423
The crystal structure of keyite, Cu3(Zn,Cu)4Cd2(AsO4)6(H2O)2, an oxysalt mineral with essential cadmium
Cooper, M. A.; Hawthorne, F. C.; The Canadian Mineralogist 34 (1996) 623–630; doi:

data_9004424
_publ_section_title
;The crystal structure of keyite, Cu3(Zn,Cu)4Cd2(AsO4)6(H2O)2, an oxysalt
 mineral with essential cadmium
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              623
_journal_page_last               630
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum            'As3 Cd Cu1.5 H4 O14 Zn2'
_chemical_name_mineral           Keyite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-I 2ya'
_symmetry_space_group_name_H-M   'I 1 2/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.11
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   11.654
_cell_length_b                   12.780
_cell_length_c                   6.840
_cell_volume                     1005.887
_database_code_amcsd             0005498
_cod_original_formula_sum        'Cu1.5 Zn2 Cd As3 O14 H4'
_cod_database_code               9004424
The crystal structure of shomiokite-(Y)
Grice, J. D.; The Canadian Mineralogist 34 (1996) 649–655; doi:

data_9004425
_publ_section_title
;
 The crystal structure of shomiokite-(Y)
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              649
_journal_page_last               655
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum            'C3 Na3 O12 Y'
_chemical_name_mineral           Shomiokite-(Y)
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P 2c -2ab'
_symmetry_space_group_name_H-M   'P b n 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   10.042
_cell_length_b                   17.349
_cell_length_c                   5.948
_cell_formula_units_Z            4
_cell_volume                     1036.253
_database_code_amcsd             0005499
_exptl_crystal_density_diffrn    2.474
_cod_original_formula_sum        'Y Na3 C3 O12'
_cod_database_code               9004425
Penobsquisite: A new borate mineral with a complex framework structure
Grice, J. D.; Gault, R. A.; Van Velthuizen, J.; The Canadian Mineralogist 34 (1996) 657–665; doi:

data_9004426
_publ_section_title
;
 Penobsquisite: A new borate mineral with a complex framework structure
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              657
_journal_page_last               665
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum            'B9 Ca2 Cl Fe H15 O23'
_chemical_name_mineral           Penobsquisite
_space_group_IT_number           4
_symmetry_space_group_name_Hall  'P 2yb'
_symmetry_space_group_name_H-M   'P 1 21 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.58
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   11.620
_cell_length_b                   9.407
_cell_length_c                   8.726
_cell_volume                     943.158
_database_code_amcsd             0005500
_exptl_crystal_density_diffrn    2.295
_cod_original_formula_sum        'Ca2 Fe Cl B9 O23 H15'
_cod_database_code               9004426
A single-crystal infrared spectroscopic and X-ray-diffraction study of untwinned San Benito perovskite containing OH groups
Beran, A.; Libowitzky, E.; The Canadian Mineralogist 34 (1996) 803–809; doi:

data_9004427
_publ_section_title
;A single-crystal infrared spectroscopic and X-ray-diffraction study of
 untwinned San Benito perovskite containing OH groups
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              803
_journal_page_last               809
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum            'Ca O3 Ti'
_chemical_name_mineral           Perovskite
_space_group_IT_number           62
_symmetry_space_group_name_Hall  '-P 2c 2ab'
_symmetry_space_group_name_H-M   'P b n m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   5.380
_cell_length_b                   5.440
_cell_length_c                   7.639
_cell_formula_units_Z            4
_cell_volume                     223.572
_exptl_crystal_density_diffrn    4.039
_cod_original_formula_sum        'Ti Ca O3'
_cod_database_code               9004427
_cod_duplicate_entry 1000022
The crystal structure of sabinaite, Na4Zr2TiO4(CO3)4
McDonald, A. M.; The Canadian Mineralogist 34 (1996) 811–815; doi:

data_9004428
_publ_section_title
;
 The crystal structure of sabinaite, Na4Zr2TiO4(CO3)4
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              811
_journal_page_last               815
_journal_volume                  34
_journal_year                    1996
_chemical_compound_source        'Mont St-Hilaire, Quebec, Canada'
_chemical_formula_sum            'C4 Na4 O16 Ti Zr2'
_chemical_name_mineral           Sabinaite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 94.14
_cell_angle_gamma                90
_cell_length_a                   10.196
_cell_length_b                   6.616
_cell_length_c                   17.958
_cell_formula_units_Z            4
_cell_volume                     1208.227
_database_code_amcsd             0005502
_exptl_crystal_density_diffrn    3.443
_cod_original_formula_sum        'Na4 Zr2 Ti C4 O16'
_cod_database_code               9004428
The atomic arrangement of Iimoriite-(Y), Y2(SiO4)(CO3)
Hughes J M; Foord E E; Jai-Nhuknan J; Bell J M; The Canadian Mineralogist 34 (1996) 817–820; doi:

data_9004429
_publ_section_title
;
 The atomic arrangement of Iimoriite-(Y), Y2(SiO4)(CO3)
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              817
_journal_page_last               820
_journal_volume                  34
_journal_year                    1996
_chemical_compound_source
'Bokan Mountain, Prince of Wales Island, Alaska, USA'
_chemical_formula_sum            'C O7 Si Y2'
_chemical_name_mineral           Iimoriite-(Y)
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                116.364
_cell_angle_beta                 92.556
_cell_angle_gamma                95.506
_cell_length_a                   6.5495
_cell_length_b                   6.6291
_cell_length_c                   6.4395
_cell_formula_units_Z            2
_cell_volume                     248.156
_database_code_amcsd             0005503
_exptl_crystal_density_diffrn    4.415
_cod_original_formula_sum        'Y2 Si C O7'
_cod_database_code               9004429
The atomic arrangement of Iimoriite-(Y), Y2(SiO4)(CO3)
Hughes J M; Foord E E; Jai-Nhuknan J; Bell J M; The Canadian Mineralogist 34 (1996) 817–820; doi:

data_9004430
_publ_section_title
;
 The atomic arrangement of Iimoriite-(Y), Y2(SiO4)(CO3)
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              817
_journal_page_last               820
_journal_volume                  34
_journal_year                    1996
_chemical_formula_sum            'C O7 Si Y2'
_chemical_name_mineral           Iimoriite-(Y)
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                116.364
_cell_angle_beta                 92.556
_cell_angle_gamma                95.506
_cell_length_a                   6.5495
_cell_length_b                   6.6291
_cell_length_c                   6.4395
_cell_formula_units_Z            2
_cell_volume                     248.156
_cod_duplicate_entry             9004429
_cod_original_formula_sum        'Y2 Si C O7'
_cod_database_code               9004430
The crystal structure of spiroffite
Cooper, M. A.; Hawthorne, F. C.; The Canadian Mineralogist 34 (1996) 821–826; doi:

data_9004431
_publ_section_title
;
 The crystal structure of spiroffite
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              821
_journal_page_last               826
_journal_volume                  34
_journal_year                    1996
_chemical_compound_source        'Moctezuma, Sonora, Mexico'
_chemical_formula_sum            'Mn2 O8 Te3'
_chemical_name_mineral           Spiroffite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 98.22
_cell_angle_gamma                90
_cell_length_a                   12.870
_cell_length_b                   5.3813
_cell_length_c                   11.888
_cell_formula_units_Z            4
_cell_volume                     814.873
_database_code_amcsd             0005504
_exptl_crystal_density_diffrn    5.059
_cod_original_formula_sum        'Te3 Mn2 O8'
_cod_database_code               9004431
Sigismundite, (Ba,K,Pb)Na3(Ca,Sr)(Fe,Mg,Mn)14Al(OH)2(PO4)12, a new Ba-rich member of the arrojadite group from Spluga Valley, Italy
Demartin, F.; Gramaccioli, C. M.; Pilati, T.; Sciesa, E.; The Canadian Mineralogist 34 (1996) 827–834; doi:

data_9004432
_publ_section_title
;
 Sigismundite, (Ba,K,Pb)Na3(Ca,Sr)(Fe,Mg,Mn)14Al(OH)2(PO4)12, a new
 Ba-rich member of the arrojadite group from Spluga Valley, Italy
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              827
_journal_page_last               834
_journal_volume                  34
_journal_year                    1996
_chemical_compound_source        'Spluga Valley, Italy'
_chemical_formula_sum
'Al0.5 Ba0.38 Ca0.94 Fe6.02 K0.06 Mg4.36 Na2.63 O50 P12 Pb0.03 Sr0.25'
_chemical_name_mineral           Arrojadite-(BaFe)
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 105.73
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   16.406
_cell_length_b                   9.945
_cell_length_c                   24.470
_cell_volume                     3842.950
_database_code_amcsd             0005505
_exptl_crystal_density_diffrn    3.125
_cod_original_formula_sum
'Al.5 Ca.94 Sr.25 Na2.63 Ba.38 K.06 Pb.03 Fe6.02 Mg4.36 P12 O50'
_cod_database_code               9004432
Magnesian hornblende from a metamorphosed ultramafic body in southwestern Finland: crystal chemistry and petrological implications
Mancini, F.; Sillanpaa, R.; Marshall, B.; Papunen, H.; The Canadian Mineralogist 34 (1996) 835–844; doi:

data_9004433
_publ_section_title
;
 Magnesian hornblende from a metamorphosed ultramafic body in southwestern
 Finland: crystal chemistry and petrological implications
;
_journal_name_full               'The Canadian Mineralogist'
_journal_page_first              835
_journal_page_last               844
_journal_volume                  34
_journal_year                    1996
_chemical_compound_source        'southwestern Finland'
_chemical_formula_sum
'Al Ca1.66 F0.2 Fe1.33 H2 K0.015 Mg3.49 Mn0.02 Na0.625 O23.8 Si7.28 Ti0.06'
_chemical_name_mineral           Hornblende
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.81
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   9.857
_cell_length_b                   18.112
_cell_length_c                   5.309
_cell_volume                     916.328
_database_code_amcsd             0005506
_exptl_crystal_density_diffrn    3.126
_cod_original_formula_sum
'Si7.28 Al Mg3.49 Fe1.33 Ti.06 Ca1.66 Na.625 Mn.02 K.015 H2 O23.8 F.2'
_cod_database_code               9004433